#------------------------------------------------------------------------------
#$Date: 2021-04-15 11:13:39 +0300 (Thu, 15 Apr 2021) $
#$Revision: 264193 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/18/1561806.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561806
loop_
_publ_author_name
'Dixon, Charlotte A.L.'
'Kavanagh, Christopher M.'
'Knight, Kevin S.'
'Kockelmann, Winfried'
'Morrison, Finlay D.'
'Lightfoot, Philip'
_publ_section_title
;
 Thermal evolution of the crystal structure of the orthorhombic perovskite
 LaFeO3
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              337
_journal_page_last               342
_journal_paper_doi               10.1016/j.jssc.2015.07.019
_journal_volume                  230
_journal_year                    2015
_chemical_formula_sum            'Fe La O3'
_chemical_formula_weight         242.75
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   5.58483(20)
_cell_length_b                   7.89328(30)
_cell_length_c                   5.58514(21)
_cell_measurement_temperature    775
_cell_volume                     246.208(16)
_computing_structure_refinement  GSAS
_pd_phase_name
'from C:/gsas/MyWork/LaFeO3GEM - Copyredone/502C/EntryWithCollCode1'
_pd_proc_ls_prof_R_factor        0.0302
_pd_proc_ls_prof_wR_factor       0.0350
_refine_ls_goodness_of_fit_all   1.88
_refine_ls_matrix_type           full
_refine_ls_number_parameters     69
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.05
_refine_ls_shift/su_mean         0.00
_cod_data_source_file            JSSC-2015-230-337.cif
_cod_data_source_block           LAFEO3GEM502C
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_geom_angle_publ_flag' value 'N' was changed to 'n' in
accordance with the built-in table derived from the CIF Core
dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21 (42 times).

data item '_geom_bond_publ_flag' value 'N' was changed to 'n' in
accordance with the built-in table derived from the CIF Core
dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21 (52 times).

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        246.208(5)
_cod_database_code               1561806
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x+1/2,+y+1/2,+z+1/2
3 +x,-y+1/2,+z
4 -x+1/2,-y,+z+1/2
-1 -x,-y,-z
-2 +x+1/2,-y+1/2,-z+1/2
-3 -x,+y+1/2,-z
-4 +x+1/2,+y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
La La1 0.02297(18) 0.25 -0.0021(5) 1.0 Uiso 0.01242(16) 4
Fe Fe1 0.0 0.0 0.5 1.0 Uiso 0.00635(9) 4
O- O1 0.4865(4) 0.25 0.0785(5) 1.0 Uiso 0.0126(5) 4
O- O2 0.27982(27) 0.03601(19) -0.27861(27) 1.0 Uiso 0.01187(27) 8
loop_
_atom_type_symbol
_atom_type_number_in_cell
La 4.0
Fe 4.0
O- 12.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O1 85.05(10) 1_555 . -2_465 n
O1 La1 O2 64.84(8) 1_555 . 1_555 n
O1 La1 O2 64.84(8) 1_555 . 3_555 n
O1 La1 O2 128.45(7) 1_555 . -2_565 n
O1 La1 O2 128.45(7) 1_555 . -4_555 n
O1 La1 O2 127.96(6) -2_566 . 1_555 n
O1 La1 O2 127.96(6) -2_566 . 3_555 n
O1 La1 O2 116.31(8) -2_566 . -2_565 n
O1 La1 O2 116.31(8) -2_566 . -4_555 n
O2 La1 O2 77.42(8) 1_555 . 3_555 n
O2 La1 O2 115.65(11) 1_555 . -2_565 n
O2 La1 O2 65.43(5) 1_555 . -4_555 n
O2 La1 O2 65.43(5) 3_555 . -2_565 n
O2 La1 O2 115.65(11) 3_555 . -4_555 n
O2 La1 O2 85.46(8) -2_565 . -4_555 n
O1 Fe1 O1 180.0 2_545 . -2_465 n
O1 Fe1 O2 88.60(9) 2_545 . 1_556 n
O1 Fe1 O2 90.41(11) 2_545 . 4_555 n
O1 Fe1 O2 91.40(9) 2_545 . -1_555 n
O1 Fe1 O2 89.59(11) 2_545 . -4_556 n
O1 Fe1 O2 91.40(9) -2_566 . 1_556 n
O1 Fe1 O2 89.59(11) -2_566 . 4_555 n
O1 Fe1 O2 88.60(9) -2_566 . -1_555 n
O1 Fe1 O2 90.41(11) -2_566 . -4_556 n
O2 Fe1 O2 91.182(19) 1_556 . 4_555 n
O2 Fe1 O2 180.0 1_556 . -1_555 n
O2 Fe1 O2 88.818(19) 1_556 . -4_556 n
O2 Fe1 O2 88.818(19) 4_555 . -1_555 n
O2 Fe1 O2 180.0 4_555 . -4_556 n
O2 Fe1 O2 91.182(19) -1_555 . -4_556 n
La1 O1 La1 104.80(9) 1_555 . -2_555 n
La1 O1 Fe1 89.98(7) 1_555 . 2_554 n
La1 O1 Fe1 89.98(7) 1_555 . 4_554 n
La1 O1 Fe1 102.29(7) -2_656 . 2_554 n
La1 O1 Fe1 102.29(7) -2_656 . 4_554 n
Fe1 O1 Fe1 154.58(14) 2_554 . 4_554 n
La1 O2 La1 98.43(8) 1_555 . -2_554 n
La1 O2 Fe1 91.56(5) 1_555 . 1_554 n
La1 O2 Fe1 88.32(6) 1_555 . 4_554 n
La1 O2 Fe1 102.54(9) -2_655 . 1_554 n
La1 O2 Fe1 98.25(10) -2_655 . 4_554 n
Fe1 O2 Fe1 158.99(7) 1_554 . 4_554 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 3.95504(20) . -1_555 n
La1 La1 3.95504(20) . -1_565 n
La1 La1 3.932(4) . -2_454 n
La1 La1 3.966(4) . -2_455 n
La1 La1 3.932(4) . -2_554 n
La1 La1 3.966(4) . -2_555 n
La1 Fe1 3.4121(24) . 1_554 n
La1 Fe1 3.4316(24) . 1_555 n
La1 Fe1 3.5248(8) . 2_454 n
La1 Fe1 3.3154(8) . 2_554 n
La1 Fe1 3.4121(24) . 3_554 n
La1 Fe1 3.4316(24) . 3_555 n
La1 Fe1 3.5248(8) . 4_454 n
La1 Fe1 3.3154(8) . 4_554 n
La1 O1 3.0299(19) . 1_455 n
La1 O1 2.6276(21) . 1_555 n
La1 O1 3.226(4) . -2_454 n
La1 O1 2.375(4) . -2_455 n
La1 O2 2.7009(19) . 1_555 n
La1 O2 2.8050(18) . 2_555 n
La1 O2 2.7009(19) . 3_555 n
La1 O2 2.8050(18) . 4_555 n
La1 O2 3.2272(19) . -1_555 n
La1 O2 2.4893(20) . -2_454 n
La1 O2 3.2272(19) . -3_555 n
La1 O2 2.4893(20) . -4_454 n
Fe1 La1 3.4316(24) . 1_555 n
Fe1 La1 3.4121(24) . 1_556 n
Fe1 La1 3.5248(8) . 2_445 n
Fe1 La1 3.3154(8) . 2_545 n
Fe1 La1 3.4121(24) . -1_555 n
Fe1 La1 3.4316(24) . -1_556 n
Fe1 La1 3.3154(8) . -2_455 n
Fe1 La1 3.5248(8) . -2_555 n
Fe1 O1 2.0229(6) . 2_545 n
Fe1 O1 2.0229(6) . -2_455 n
Fe1 O2 2.0129(20) . 1_556 n
Fe1 O2 2.0036(19) . 4_555 n
Fe1 O2 2.0129(20) . -1_555 n
Fe1 O2 2.0036(19) . -4_455 n
O1 La1 2.6276(21) . 1_555 n
O1 La1 3.0299(19) . 1_655 n
O1 La1 3.226(4) . -2_554 n
O1 La1 2.375(4) . -2_555 n
O1 Fe1 2.0229(6) . 2_554 n
O1 Fe1 2.0229(6) . 4_554 n
O2 La1 2.7009(19) . 1_555 n
O2 La1 2.8050(18) . 2_544 n
O2 La1 3.2272(19) . -1_555 n
O2 La1 2.4893(20) . -2_554 n
O2 Fe1 2.0129(20) . 1_554 n
O2 Fe1 2.0036(19) . 4_554 n
